# Modelling microfibril angle variation in New Zealand-grown radiata pine

- John R Moore
^{1}Email author, - Dave J Cown
^{1}and - Russell B McKinley
^{1}

**44**:25

https://doi.org/10.1186/s40490-014-0025-4

© Moore et al.; licensee Springer. 2014

**Received: **29 May 2014

**Accepted: **30 September 2014

**Published: **17 October 2014

## Abstract

### Background

Microfibril angle (MFA) is a property of wood cell walls that has a strong influence on end-product quality, particularly for solid timber. Forest managers, tree breeders and wood processors require more quantitative information on the inter- and intra-stem variation in MFA in order to understand the impacts of their decisions on wood quality. The aim of this study was to develop parametric models that can be used to predict the intra- and inter-stem variation in MFA in radiata pine (*Pinus radiata* D. Don) trees growing in New Zealand

### Methods

Empirical models were developed using a dataset that contained records from 347 trees in which radial profiles of MFA have been measured at different heights up the stem. Radial variation in MFA was modelled as a function of cambial age using both a modified logistic function and a modified Michaelis-Menten equation. Additional terms were added to these models to account for differences in MFA with relative height up the stem.

### Results

Values of MFA ranged from more than 40° near the pith to approximately 10-15° in the outerwood. Values greater than 30° were largely confined to the inner rings of the butt logs. A variance components analysis showed that most of the variation in MFA occurred within stems, with less than 15% of the variation due to differences between sites. The final models were able to account for 57-63% of the variation in MFA and inclusion of a relative height term significantly improved the model fit.

### Conclusions

Radiata pine has a region of high microfibril angle in the first 10-15 growth rings from the pith, particularly at the base of the tree. Growth rate had a small positive influence on average MFA (wider rings resulting in higher MFA values). Site differences were small, indicating that regional variation in wood stiffness is due more to the known trends in wood density. The models developed here can be coupled to growth models to examine how the combination of site productivity and silvicultural regime affect the size of the central zone containing high MFA wood.

### Keywords

Microfibril angle Wood properties Radiata pine Radial variation Ultrastructure## Background

The mechanical and physio-mechanical properties (mainly stiffness, shrinkage and stability) of wood are determined by the fundamental structure of its cells (Barnett and Bonham [2004]; Cave [1969]; Harris and Meylan [1965]; McLean et al. [2010]; Wardrop and Preston [1947]). Studies in radiata pine (*Pinus radiata* D. Don) and other softwood species have shown that the two most influential wood properties are basic density and the angle of the cellulose microfibrils (MFA) in the S2 layer of wood cell walls (Cown et al. [1999]; Donaldson [1997]; Wagner et al. [2012]; Walker and Butterfield [1995]; Walker [1996]; Xu and Walker [2004]). Microfibril angle has been considered so important that several authors have proposed using it as a criterion for differentiating juvenile and mature wood (Clark et al. [2006]; Mansfield et al. [2009]). Longitudinal shrinkage and stiffness of radiata pine wood (and in wood of other species) are adversely correlated with high MFA (Astley et al. [1998a], [b]; Evans et al. [2001]), which has negative consequences for the utilisation of the wood from parts of a tree where there is high MFA. However, there is only general information describing the variation in MFA within and between trees. Few, if any, empirical models exist that are able to quantify the patterns of variation that are observed in radiata pine MFA. This is partly due to difficulties in collecting large datasets on MFA variation using many of the early measurement techniques, which were based on microscopy and were relatively slow (Batchelor et al. [1997]; Donaldson [2008]; Verbelen and Stickens [1995]). However, other methods such as near-infrared spectroscopy (Schimleck and Evans [2002]) and X-ray diffraction (Cave [1966], [1997]; Evans [1999]) enable data on MFA to be more readily collected on large numbers of samples. The latter method is widely used due to automation and the possibility of increased resolution of measurements of within-growth ring variation (Evans et al. [2001]).

Previous studies that investigated the within-tree variation in MFA found that very large values of MFA (circa 45°) are common in the innermost growth rings (Donaldson [2008]). These values decrease rapidly across the corewood zone, which generally constitutes the first 10 to 15 growth rings from the pith (Cown [1992]), before stabilising at values of 10-15° in the outerwood. For a given cambial age, values of MFA decline with increasing distance up the stem and the rate of decline in MFA with increasing cambial age is also generally lower further up the stem. The value of MFA has also been found to stabilise at an earlier cambial age further up the stem (Butterfield [1997]; Cave and Walker [1994]; Cown et al. [2004]; Donaldson [1992], [1993]; Evans et al. [2001]; Watt et al. [2011]). Similar within-tree patterns in MFA have been observed in a number of other conifer species (Auty et al. [2013]; Jordan et al. [2005]; Mansfield et al. [2009]; Megraw [1998]) and also in hybrid poplars (Fang et al. [2006]). High values of MFA that are observed near the pith have been hypothesised to provide young trees with the flexibility to bend through large angles, in response to wind and snow loading, without breaking (Barnett and Bonham [2004]; Booker and Sell [1998]; Lichtenegger et al. [1999]).

More quantitative information on the variation in MFA within and between trees is required by forest managers and wood processors in order to understand the implications of past and proposed silvicultural practices on the quality of the forest resource. For example, the reduction in rotation length and the move to more widely spaced stands has resulted in trees with a greater proportion of juvenile wood with high MFA, low stiffness and high longitudinal shrinkage (Zobel and Sprague [1998]). Wider tree spacing also results in an increase in radial growth rates, which can be further enhanced through treatments such as fertilisation and weed control. Research in other species has shown that treatments which enhance radial growth can affect MFA (Lindström et al. [1998]; Lundgren [2004]; Sarén et al. [2004]). Therefore, it is important to determine whether MFA is simply a function of cambial age or whether it is also affect by rate of growth as expressed through growth ring width. Developing higher resolution wood property models that are ultimately able to be linked to growth models is a constructive step towards better understanding the effects of factors such as site and silviculture on end product performance (Houllier et al. [1995]; Kellomaki et al. [1999]; Leban et al. [1996]; Seifert [1999]).

Models for the radial and vertical trends in MFA have been developed for loblolly pine (*Pinus taeda* L.) (Jordan et al. [2005], [2007]), Scots pine (*Pinus sylvestris* L.) (Auty et al. [2013]), lodgepole pine (*Pinus contorta* var. *latifolia* Doug. ex Loud.) (Wang and Stewart [2012]) and *Acacia mangium* (Abdullah et al. [2010]; Tabet et al. [2012]), where cambial age and height in the stem have been identified as the main contributors to variation. An early attempt to describe MFA variation in radiata pine was a model based on data from polarised light studies (Tian and Cown [1995]). Since the development of this early model, considerable amounts of data have been collected on radiata pine MFA. Most of these data have been collected using the SilviScan instrument (Evans et al. [2000]). Ring-level data are now available from different heights in the stem for trees growing across the range of site types where radiata pine typically grows in New Zealand. Using available data on radiata pine MFA, the overall objectives of this study were to: (1) quantify the extent of variation in MFA within and between trees; (2) develop empirical models that are able to explain the observed intra-stem patterns in MFA; and (3) and to determine whether observed radial patterns are affected by growth rate.

## Methods

### Data sources

**Summary of the studies in which microfibril angle data were collected**

Site No. | Region | Forest | Age (yrs) | n (trees) | Sample heights (m) |
---|---|---|---|---|---|

1 | Auckland | Aupouri | 25 | 10 | 0, 1.4, 5, 20 |

2 | Auckland | Mangakahia | 23 | 40 | 0, 1.4, 5, 20 |

3 | Auckland | Athenree | 25 | 10 | 0,1.4, 5,10,15,20,25 |

4 | Auckland | Woodhill | 33 | 20 | 1.4 |

5 | Rotorua | Kaingaroa | 18 | 20 | 1.4 |

6 | Rotorua | Kaingaroa | 18 | 20 | 1.4 |

7 | Rotorua | Kaingaroa | 25 | 25 | 0, 5, 10 |

8 | Rotorua | Kaingaroa | 25 | 10 | 0, 1.4, 5, 20 |

9 | Rotorua | Kaingaroa | 25 | 10 | 0, 1.4, 5, 20 |

10 | East Coast | Ruatoria | 25 | 10 | 0, 1.4, 5, 20 |

11 | Hawkes Bay | Mohaka | 25 | 10 | 0, 1.4, 5, 20 |

12 | Wellington | Lismore | 25 | 6 | 0, 1.4, 5, 20 |

13 | Wellington | Ngaumu | 25 | 10 | 0, 1.4, 5, 20 |

14 | Nelson | Wyeburn - Marlborough | 18 | 20 | 1.4 |

15 | Nelson | Lansdowne - Marlborough | 18 | 20 | 1.4 |

16 | Nelson | Golden Downs | 25 | 25 | 0, 5, 10 |

17 | Nelson | Rabbit Island | 25 | 10 | 0, 1.4, 5, 20 |

18 | Nelson | Golden Downs | 25 | 10 | 0, 1.4, 5, 20 |

19 | Nelson | Waimea | 25 | 10 | 0, 1.4, 5, 20 |

20 | Nelson | Golden Downs | 33 | 7 | 1.4 |

21 | Canterbury | Ashley | 25 | 9 | 0, 1.4, 5, 20 |

22 | Canterbury | Eyrewell | 25 | 10 | 0, 1.4, 5, 20 |

23 | Canterbury | Waimate | 25 | 10 | 0, 1.4, 5, 20 |

24 | Southland | Blackmount - Southland | 25 | 2 | 0, 1.4, 5, 20 |

25 | Southland | Rowallan - Southland | 25 | 7 | 0, 1.4, 5, 21 |

26 | Southland | Longwood - Southland | 25 | 6 | 0, 1.4, 5, 22 |

Total tree height measurements were absent in most studies. Because of the different ages in the dataset and the need to be able to predict the intra-stem patterns in MFA for a wide range of tree sizes, it is helpful to know the relative height that each sample was taken from as well as the absolute height. To overcome the problem of missing heights, total height was predicted for each tree using a compatible volume and taper function along with data on the diameter and heights of each disc sampled from the tree. For each tree, the estimated value of total height was adjusted incrementally and the difference between the actual and predicted diameters of the discs determined. The predicted height of each tree was selected, such that the difference between actual and predicted disc diameters was minimised (Appendix 1). When tested using a dataset where total tree height was known, this approach was able to predict tree height to within 5% of the measured value. The relative height that each disc was sampled from was estimated by dividing the absolute sampling height by the predicted height of the corresponding tree.

### Data analyses

Because the data had a hierarchical structure (i.e. growth rings within discs, within trees, within stands), a mixed-modelling approach was adopted to ensure that appropriate estimates of parameter standard errors were obtained and tests of parameter significance were valid (Pinheiro and Bates [2000]). A variance components analysis was undertaken using Restricted Maximum Likelihood to determine how much of the variation in MFA was attributable to each stratum (i.e., site, tree, disc or ring) in the dataset. A number of different model forms were then evaluated for their ability to explain the radial trends in MFA. Once the most suitable model form was identified, the second step was to determine whether the model parameters varied as a function of height within the tree. Model selection was based on visual analysis of plots of the normalised residuals versus fitted and explanatory variables (Pinheiro and Bates [2000]) and Akaike's information criterion (AIC, (Akaike [1974])), which measures the relative adequacy of different nested models. Akaike's information criterion is used when comparing models fitted to the same dataset and the model with the lower AIC is generally preferred. Parameter estimates were obtained using the maximum-likelihood method, and only those parameters that were significant (*p* < 0.05) were retained in the final models. Two sets of fit indices (*R*^{2}) were calculated using the equations given in Parresol (Parresol [1999]). In the first set, the predicted values were estimated from only the fixed-effects terms of each model, and in the second, they were calculated from both the fixed and random effects. All statistical analyses were carried out using functions contained in the nlme library (Pinheiro et al. [2012]) of the R statistical programming environment (R Development Core Team [2013]).

where *y*_{
ijkl
} is the mean MFA (degree) in each annual growth ring, *CA*_{
ijkl
} is the cambial age (years) of the *l*^{th} annual ring of the *k*^{th} disc from the *j*^{th} tree at the *i*^{th} site, *α*_{0}, *α*_{1} and *α*_{2} are fixed effects parameters to be estimated, representing the initial value near the pith, the rate parameter and the lower asymptote, respectively; *ε*_{
ijkl
} is the random error due to the *l*^{th} annual ring of the *k*^{th} disc from the *j*^{th} tree at the *i*^{th} site. Since *α*_{2} assumes a constant value across all cambial ages, this parameter was allowed to vary randomly in each stratum. Hence, *a*_{2,i}, *a*_{2,ij} and *a*_{2,ijk} represent the random effects of the *i*^{th} site, the *j*^{th} tree from the *i*^{th} site, and *k*^{th} disc from the *j*^{th} tree from the *i*^{th} site, respectively.

where *RW*_{
ijkl
} is the width (millimetres) of the *l*^{th} annual ring of the *k*^{th} disc from the *j*^{th} tree at the *i*^{th} site, *β*_{01}, *β*_{02}, *β*_{1} and *β*_{2} are the fixed effects parameters to be estimated. In this equation, *β*_{1} represents the rate parameter and *β*_{2} the intercept, while the lower asymptote is given by *β*_{1} + *β*_{2}. The random effects of the *i*^{th} site, *j*^{th} tree in *i*^{th} site and *k*^{th} disc from *j*^{th} tree in *i*^{th} site are given by *b*_{
2,i
}, *b*_{
2,ij
} and *b*_{
2,ijk
}, respectively. In order to incorporate the increasing influence of ring width at higher cambial ages, the *β*_{0} parameter was allowed to vary as a function of ring width. This had the effect of changing the asymptotic mature wood value of MFA without altering the initial value near the pith.

In fitting the models to the data, heteroscedasticity was modelled as a power function of the absolute values of cambial age, while a first-order autoregressive correlation structure AR(1) was applied to model correlation among observations at successive cambial ages within each grouping factor. More details about these variance and autocorrelation functions are given in Auty et al. ([2013]) and Jordan et al. ([2005]).

For both models, the fixed-effects parameters were also modified to include possible effects of height up the stem. Linear, log-linear and quadratic relative height terms were added to the models given by Eqs. (1) and (2) following the approach described in Jordan et al. ([2005]). For terms involving the natural logarithm of relative height, a small value (0.1) was added to the relative height term to avoid zero values, which would have resulted in infinite values when the natural logarithm of this term was taken.

In order to visualise the intra-stem pattern in MFA, the models were then applied to a single 29-year-old tree (DBH = 32.8 cm, height = 36.9 m) that had spatial information on ring number from the pith generated at 5 mm resolution in the radial direction and 100 mm resolution in the longitudinal direction. This information was generated using the Forecaster growth and yield modelling system (West et al. [2013]).

## Results

**AIC, log-likelihood and fit indices for the models to predict MFA given by Eqs. 1 & 2**

**Parameter estimates and associated standard errors (s.e.) and tests of significance for the models given by Eq.** (1) **and Eq (2)**

### Modelling variation with height

_{rel}) to each of the parameters in the modified logistic function (see Eq. (3)) resulted in a significant improvement in the model fit and all the height terms were significant. Quadratic terms for HT

_{rel}were added to the model (results not shown) and these were found to be significant, but the resulting predictions of MFA were found to be non-plausible, so these terms were dropped. The natural logarithm of HT

_{rel}+ 0.1 was also found to be significant in the model, with the exception of the term added to the lower asymptote (

*α*

_{5}) (Eq. 4). The model given by Eq. (3) was able to explain 62% of the variation in MFA based on the fixed effects alone (78% when the random effects of site, tree and disc were included) (Table 4). The modified logistic equation with log

*HT*

_{ rel }terms added (Eq. 4) performed slightly better and was able to explain 65% of the variation in MFA (81% when the random effects of site, tree and disc were included). The parameter estimates for the two models are given in Table 5.

**AIC, log-likelihood and fit indices for the models to predict MFA given by Eqs. 3-6**

**Parameter estimates and associated standard errors (s.e.) and tests of significance for the models given by Eqs.** (6)-(9)

Parameter | Estimate | s.e. | t-value | p-value |
---|---|---|---|---|

Eq. (6) | ||||

| 50.510 | 0.423 | 119.295 | <0.001 |

| 0.148 | 0.002 | 69.569 | <0.001 |

| 13.209 | 0.457 | 28.877 | <0.001 |

| −51.438 | 2.625 | −19.596 | <0.001 |

| 0.503 | 0.027 | 18.576 | <0.001 |

| 2.069 | 0.510 | 4.060 | <0.001 |

Eq. (7) | ||||

| 15.275 | 1.117 | 13.674 | <0.001 |

| 0.335 | 0.010 | 34.670 | <0.001 |

| 13.458 | 0.451 | 29.871 | <0.001 |

| −16.783 | 0.588 | −28.566 | <0.001 |

| 0.082 | 0.004 | 18.410 | <0.001 |

Eq. (8) | ||||

| −32.156 | 0.418 | −76.850 | <0.001 |

| 3.663 | 0.138 | 26.494 | <0.001 |

| 40.178 | 0.657 | 61.124 | <0.001 |

| 0.518 | 0.008 | 67.041 | <0.001 |

| −5.462 | 0.556 | −9.818 | <0.001 |

Eq. (9) | ||||

| −32.109 | 0.407 | −78.874 | <0.001 |

| 3.718 | 0.140 | 26.509 | <0.001 |

| 36.190 | 0.710 | 50.987 | <0.001 |

| 0.517 | 0.008 | 66.477 | <0.001 |

| −1.895 | 0.154 | −12.310 | <0.001 |

*HT*

_{ rel }) terms were also found to be significant when added to the Michaelis-Menten equation (Eqs. 5 & 6). The models given by Eqs. 5 and 6 were able to explain 59 and 62% of the variation in MFA, respectively (Table 4). Parameter estimates for the two models are given in Table 4. Based on the goodness of fit statistics (Table 5), it appears that the model given by Eq. (4) is able to explain the greatest amount of variation in MFA, although all four models perform similarly.

### Visualisation of model predictions

*HT*

_{ rel }) appears to give a more realistic representation of the low stiffness core at all heights in the tree than the model simply based on

*HT*

_{ rel }, but the predicted low stiffness zone at the base of the tree is not as severe (Figure 2a and b). The predictions from the two Michaelis-Menten equations were very similar to each other (Figure 2c and d), but indicated that the high MFA zone extended much higher in the stem than the modified logistic model.

## Discussion

Despite the acknowledged influence of MFA on wood performance, there is relatively little information on the factors influencing its magnitude (apart from cambial age and height in the stem) in comparison to wood properties such as density. This is not altogether surprising as the analyses undertaken in this study showed that approximately 82% of the variation in MFA was in the longitudinal and radial directions within the stem, with less than 15% of the variation occurring among sites. The level of variation between sites was much higher than the 2% found for Scots pine by Auty et al. ([2013]), but lower than that found in loblolly pine (Jordan et al. [2006]). These differences presumably reflected the relative distribution of sites sampled in New Zealand compared with these other two studies. While site-level variation was relatively small, it is still considered worthwhile to investigate this further as previous studies have shown that MFA is affected by exposure to wind (Telewski [1989]) and mean temperature during the growing season (Cortini et al. [2014]). Other site factors, such as soil type and rainfall distribution, may also be important, particularly when studies have shown that irrigation and fertilisation can increase MFA (Downes et al. [2002]; Wimmer et al. [2002]). Previous studies have also shown that there are genetic differences in MFA in radiata pine and other species (Donaldson [1993]; Vainio et al. [2002]), while it has also been shown to be a moderately heritable trait (Baltunis et al. [2007]; Burdon and Low [1992]; Dungey et al. [2006]; Gapare et al. [2007]; Jayawickrama [2001]; Wu et al. [2008]). The genetic origin of the study trees is very diverse, with many originating from open-pollinated families, and this is likely to have accounted for some of the unexplained variation in the models (Cortini et al. [2014]). There are several large-plot trials in New Zealand that contain trees from different, but known, genetic origins (e.g. Carson et al. [1999]), which could provide potential future opportunities to investigate genetic differences in radiata pine MFA in more detail.

The models developed here have quantified much previous knowledge about intra-stem variation in MFA. Visualisations of the two-dimensional patterns in MFA highlight the issue of juvenile wood (corewood) in radiata pine, which in addition to having high MFA also has low wood density and high spiral grain angle (Burdon et al. [2004]; Cown [1992]). Solid timber cut from this part of the tree will inevitably have low stiffness because of low density and high MFA, and a high propensity to twist because of high spiral grain (Cown et al. [2010]), so will be unsuitable for many appearance and structural applications. It is clear from this and other studies that high microfibril angle is a characteristic feature of the juvenile core of radiata pine and many conifers, and it is adversely affected by increased growth rates (Dumbrell and McGrath [2000]; Herman et al. [1999]; Sarén et al. [2004]; Watt et al. [2011]). The impact of the presence of juvenile wood is exacerbated by the positive relationship between growth rate and MFA. This presents a challenge since silviculture in New Zealand has traditionally favoured rapid diameter growth – so not only is the core larger, but its properties are poorer. However, if increasing site productivity is the main goal of forest management there are options for increasing overall volume while restraining individual stem growth. Unfortunately, it is very difficult to restrict the size of the juvenile core and the overall proportion of juvenile wood through spacing, except at the extremes (West [1997]), but more conservative thinning may give more uniform final crops with better average stem form, smaller branches and less radial variation in wood properties. Silvicultural influences on the distributions of internal wood properties were not examined in this study, but analysis of data from replicated silvicultural trials has shown that tree spacing does have a significant influence on MFA (Lasserre et al. [2009]; Watt et al. [2011]). Therefore, while increased stand density may not reduce the size of the juvenile wood zone and the overall proportion of juvenile wood, it may improve the properties of the wood found in the first 10-15 growth rings from the pith.

Stiffness variation is best explained by a combination of MFA and wood density (Cown et al. [1999]; Downes et al. [2002]; Megraw et al. [1999]). Given that site-level variation in MFA is relatively small, we hypothesise that regional differences in modulus of elasticity that are observed across New Zealand (Watt and Zoric [2010]) are driven by differences in wood density (Palmer et al. [2013]), rather than site-level differences in MFA. This hypothesis will be further tested using data from a subset of 17 sites which contain trees from the same seedlot, grown under the same silvicultural regime, and where data were collected on density, MFA and SilviScan-derived modulus of elasticity. Detailed information of soil properties and climate are also available, which will permit further investigation into possible explanatory variables responsible for site-level variation.

The models developed in this study are intended to be coupled to a growth model which enables the effects of different management practices and site productivity on the microfibril angle distribution and the size of this corewood zone to be examined. There are two important issues to consider here. Firstly, the models need to be tested against data from stands with contrasting growth rates, e.g. stands established at different densities or thinned to different densities. Factors such as crown size and shape also need to be considered as these might help to explain additional variation in MFA. Most of the data used to develop the models came from stands that had received similar silvicultural treatments and, therefore, their ability to accurately predict the effects of treatments such as thinning and pruning is untested. Secondly, forest managers who use such systems require an objective way to compare trees grown under different regimes. One way to do this would be to determine the proportion of the cross-sectional area of a disc or the volume of a log that has values of MFA above a certain threshold (say, 15°). This would also provide a quantitative measure that forest managers could use to compare regimes.

There are several limitations to the data used to develop the models as well as the models themselves. Firstly, some caution should be exercised when interpreting the longitudinal trends in MFA within a stem, particularly in the uppermost part of the stem, as most of the data were collected from below 60% of relative height. Secondly, total height was not directly measured on the vast majority of sample trees, but was instead predicted from sectional measurements made along the stem. While this has introduced another potential source of error into the data, it is unlikely to have manifestly affected the results obtained from this study. However, the authors strongly recommend that tree height is measured in all future wood quality studies to better enable modelling of the intra-stem distribution of wood properties and to enable the mechanisms by which silvicultural treatments alter these properties to be elucidated. Thirdly, the data were collected from only a single pith-to-bark radial sample from each selected height along the stem. Therefore, potential circumferential variation in MFA is unknown and cannot be included in the model, although one study has suggested that this is not a significant source of error (Hein and Brancheriau [2011]). A recently developed automated system (Emms and Hosking [2006]) is able to provide information on the three-dimensional MFA variation within a wood disc, and hence within complete stems. The system measures the ultrasonic velocity in the longitudinal direction, which is strongly and negatively correlated with MFA determined by X-ray diffraction (Scion, unpublished data). Finally, the "best" models developed in this study were able to explain about 60% of the variation in MFA. The 40% unexplained variation is important as it is hypothesised that it is this variation, when superimposed on top of the explained variation (explained by the types of models developed in this study) which drives end product performance (Jonathan Harrington, Scion – pers. comm). More detailed analyses are needed to understand this variation and to be able to account for it in wood properties models, possibly through the introduction of random perturbations to the predictions from the models developed in this study.

## Conclusions

This study summarises one of the most comprehensive datasets on MFA for a single species anywhere in the world. Approximately 82% of the total variation in MFA was due to differences within the stem of a tree, with less than 15% due to differences among sites. This intra-stem variation could be modelled as a function of cambial age and relative height within the stem, with the "best" models explaining about 60% of the variation in MFA. Like many other conifer species, radiata pine has a region of high microfibril angle in the first 10-15 growth rings from the pith, particularly at the base of the tree. Because of the silvicultural regimes that radiata pine is grown under (i.e. relatively wide initial spacing and short rotation lengths) the volume occupied by this high MFA wood is relatively high. The models developed in this study are able to be coupled to growth models enabling the impacts of site productivity and silvicultural regimes on the MFA distribution with a tree to be investigated.

## Authors' contributions

JRM conceived the idea for the overall analysis of available data, undertook the data analysis and writing of the manuscript. DJC and RBMcK planned most of the wood quality assessments and contributed to the interpretation of the results and writing of the manuscript. All authors read and approved the final version of the manuscript.

## Appendix – Derivation of method to estimate tree height from sectional measurements

*d*is the inside bark diameter (cm) at height

*h*(m) above the ground;

*V*is the volume equation

*k* is $\frac{\pi}{4}\times {10}^{-4}$, the constant for converting square diameter to basal area; *H* is total height (m) with 1.4 being breast height; *D* is outside bark diameter at breast height in cm; *X* is $\left(\frac{H-h}{H}\right)$; and *α*_{1} to *α*_{3} and *β*_{1} to *β*_{9} are equation coefficients.

Different sets of coefficients for Equation [A1] were available, including local coefficients specific to many of the forests where MFA data were collected. The compatible volume and taper equation for the direct sawlog regime developed by Katz et al. ([1984]) generally performed better than the local taper and volume functions, and hence was used to estimate the heights of trees in all forests.

The total height *H*, of a given tree, was numerically estimated from Equation [1] by searching for the value of *H* that gave a taper curve that minimised the sum of squared residuals given the observed diameters and heights above ground of the discs from the tree. This was achieved by use of a SAS macro that had been programmed to search across a range of total height values (0.5 m above the height above ground of the topmost disc to a distance of 60 m beyond this starting point), at intervals of 0.01 m, and return the value of *H* corresponding to the minimised sum of squared residuals. An evaluation of this approach showed that the total height estimates were generally reasonable. However, it was possible that total heights of a few of the trees were overestimated as their height estimates were beyond the expected maximum values for radiata pine trees of a given age. Graphical plots of the taper equations of best fit (not shown), overlain on the disc diameter and height data from select trees across the range of tree dbh in the data, also showed that the total heights of the larger diameter trees were slightly overestimated, especially those trees where diameter at breast height was greater than 50 cm the topmost disc was sampled at only 10 m above the ground.

## Declarations

### Acknowledgments

The authors wish to acknowledge Wood Quality Initiative Ltd. who funded several of the studies where MFA data were collected and for allowing publication of the results. Funding for publication of the results was also provided by Future Forests Research Ltd. Dr Paul Kibblewhite provided access to data from earlier studies looking at MFA variation in different radiata pine clones. Dr Charles Sabatia provided assistance with the statistical analysis of the data. Dr David Auty provided advice on the modelling and presentation of the results. Four anonymous reviewers provided useful comments on an earlier version of this manuscript.

## Authors’ Affiliations

## References

- Abdullah N, Tabet T, Aziz F:
**Regression models on the age-affecting and microfibril angle of**Acacia mangium**.***Journal of the Indian Acadamy of Wood Science*2010,**7**(1–2):49–53. doi:10.1007/s13196–011–0010-y 10.1007/s13196-011-0010-yView ArticleGoogle Scholar - Akaike H:
**A new look at the statistical model identification.***IEEE Transactions on Automatic Control*1974,**19:**716–723. 10.1109/TAC.1974.1100705View ArticleGoogle Scholar - Astley RJ, Harrington JJ, Tang S, Neumann J:
**Modelling the Influence of Microfibril Angle on Stiffness and Shrinkage in Radiata Pine.**In*Microfibril Angle in Wood. Proc. IAWA/IUFRO International Workshop on the Significance of Microfibril Angle to Wood Quality*. Edited by: Butterfield BG. University of Canterbury, Christchurch, New Zealand; 1998a:272–295.Google Scholar - Astley RJ, Stol KA, Harrington JJ:
**Modelling the elastic properties of softwood. Part II: the cellular microstructure.***Holz als Roh- und Werkstoff*1998,**56**(1):43–50. 10.1007/s001070050262View ArticleGoogle Scholar - Auty D, Gardiner BA, Achim A, Moore JR, Cameron AD:
**Models for predicting microfibril angle variation in Scots pine.***Annals of Forest Science*2013,**70:**209–218. 10.1007/s13595-012-0248-6View ArticleGoogle Scholar - Baltunis BS, Wu HX, Powell MB:
**Inheritance of density, microfibril angle, and modulus of elasticity in juvenile wood of**Pinus radiata**at two locations in Australia.***Canadian Journal of Forest Research-Revue Canadienne De Recherche Forestiere*2007,**37**(11):2164–2174. doi:10.1139/X07–061 10.1139/X07-061View ArticleGoogle Scholar - Barnett JR, Bonham VA:
**Cellulose microfibril angle in the cell wall of wood fibres.***Biological Reviews of the Cambridge Philosophical Society*2004,**79**(2):461–472. 10.1017/S1464793103006377View ArticlePubMedGoogle Scholar - Batchelor WJ, Conn AB, Parker IH:
**Measuring the fibril angle of fibres using confocal microscopy.***Appita*1997,**50:**377–380.Google Scholar - Booker RE, Sell J:
**The nanostructure of the cell wall of softwoods and its functions in a living tree.***Holz Als Roh-Und Werkstoff*1998,**56**(1):1–8. doi:10.1007/s001070050255 10.1007/s001070050255View ArticleGoogle Scholar - Burdon RD, Kibblewhite RP, Walker JCF, Megraw RA, Evans R, Cown DJ:
**Juvenile versus mature wood: a new concept, orthogonal to corewood versus outerwood, with special reference to**Pinus radiata**and**P. taeda**.***Forest Science*2004,**50**(4):399–415.Google Scholar - Burdon RD, Low CB:
**Genetic survey of**Pinus radiata**. 6. Wood properties: variation, heritabilities, and interrelationships with other traits.***New Zealand Journal of Forestry Science*1992,**22:**228–245.Google Scholar - Butterfield BG:
*Microfibril angle in wood. (Eds.), Proceedings of the IAWA/IUFRO International Workshop on the Significance of Microfibril Angle to Wood Quality; Westport, University of Canterbury*. 1997.Google Scholar - Carson SD, Kimberley MO, Hayes JD, Carson MJ:
**The effect of silviculture on genetic gain in growth of**Pinus radiata**at one-third rotation.***Canadian Journal of Forest Research*1999,**29**(12):1979–1984. doi:10.1139/x99–152 10.1139/x99-152View ArticleGoogle Scholar - Cave ID:
**X-ray measurement of microfibril angle.***Forest Products Journal*1966,**16:**37–42.Google Scholar - Cave ID:
**The longitudinal Young's modulus of**Pinus radiata**.***Wood Science and Technology*1969,**3**(1):40–48. 10.1007/BF00349983View ArticleGoogle Scholar - Cave ID:
**Theory of X-ray measurement of microfibril angle in wood Part 1. The condition for reflection X-ray diffraction by materials with fibre type symmetry.***Wood Science and Technology*1997,**31**(3):143–152. 10.1007/BF00705881View ArticleGoogle Scholar - Cave ID, Walker JCF:
**Stiffness of wood in fast-grown plantation softwoods.***Forest Products Journal*1994,**44**(5):42–48.Google Scholar - Clark A, Daniels RF, Jordan L:
**Juvenile/mature wood transition in loblolly pine as defined by annual ring specific gravity, proportion of latewood, and microfibril angle.***Wood and Fiber Science*2006,**38**(2):292–299.Google Scholar - Cortini, F, Groot, A, Tong, Q, & Duchesne, I. (2014). Ring-level models for predicting wood and fibre properties of Abies balsamea. Wood Science and Technology, doi:10.1007/s00226–014–0664-x.Google Scholar
- Cown DJ:
**Corewood (juvenile wood) in**Pinus radiata**- should we be concerned?***New Zealand Journal of Forestry Science*1992,**22**(1):87–95.Google Scholar - Cown DJ, Ball RD, Riddell MJC:
**Wood density and microfibril angle in 10**Pinus radiata**clones: distribution and influence on product performance.***New Zealand Journal of Forestry Science*2004,**34**(3):293–315.Google Scholar - Cown, DJ, Harrington, J, Bourreau, D, Haug, J, & Lee, J (2010). Spatial variation in spiral grain: a single stem of
*Pinus radiata*D.Don.*New Zealand Journal of Forestry Science, 40*, 211–224.Google Scholar - Cown DJ, Hebert J, Ball R:
**Modelling**Pinus radiata**lumber characteristics. Part 1: mechanical properties of small clears.***New Zealand Journal of Forestry Science*1999,**29**(2):203–213.Google Scholar - Donaldson LA:
**Within- and betwee-tree variation in microfibril angle in**Pinus radiata**.***New Zealand Journal of Forestry Science*1992,**22:**77–86. 10.1080/03036758.1992.10420807View ArticleGoogle Scholar - Donaldson LA:
**Variation in microfibril angle among three genetic groups of**Pinus radiata**trees.***New Zealand Journal of Forestry Science*1993,**23:**90–100.Google Scholar - Donaldson LA:
**Microfibril angle - its influence on wood properties, and prospects for improvement in radiata pine.**In*Wood Quality Workshop '95*. Edited by: Klitscher K, Cown D, Donaldson L. New Zealand Forest Research Institute, Rotorua, New Zealand; 1997. (pp. 20–25, FRI Bulletin No. 201)Google Scholar - Donaldson LA:
**Microfibril angle: measurement, variation and relationships - a review.***IAWA Journal*2008,**29**(4):345–386. 10.1163/22941932-90000192View ArticleGoogle Scholar - Downes GM, Nyakuengama JG, Evans R, Northway R, Blakemore P, Dickson RL, Lausberg M:
**Relationship between wood density, microfibril angle and stiffness in thinned and fertlized**Pinus radiata**.***IAWA Journal*2002,**23**(3):253–265. 10.1163/22941932-90000302View ArticleGoogle Scholar - Dumbrell IC, McGrath JF:
**Effect of fertiliser and growth rate on angle of spiral grain in young**Pinus radiata**in Western Australia.***Australian Forestry*2000,**63**(2):142–146. 10.1080/00049158.2000.10674824View ArticleGoogle Scholar - Dungey HS, Matheson AC, Kain D, Evans R:
**Genetics of wood stiffness and its component traits in**Pinus radiata**.***Canadian Journal of Forest Research*2006,**36**(5):1165–1178. 10.1139/x06-014View ArticleGoogle Scholar - Emms GW, Hosking C:
**Mapping the stiffness properties in trees.***Scion Wood Processing Newsletter*2006,**39:**2pp.Google Scholar - Evans R:
**Variance approach to the X-ray diffractometric estimation of microfibril angle in wood.***Appita Journal*1999,**52**(4):283–294.Google Scholar - Evans R, Booker R, Kibblewhite RP:
*Variation of Microfibril Angle, Density and Stiffness in Fifty Radiata Pine Trees*. 2001.Google Scholar - Evans R, Hughes M, Menz D:
**Microfibril angle variation by scanning X-ray diffractometry.***Appita Journal*1999,**52**(5):363–367.Google Scholar - Evans R, Ilic J, Matheson C:
*Rapid Estimation of Solid Wood Stiffness using SilviScan*. 2000.Google Scholar - Fang S, Yang W, Tian Y:
**Clonal and within-tree variation in microfibril angle in poplar clones.***New Forests*2006,**31**(3):373–383. 10.1007/s11056-005-8679-7View ArticleGoogle Scholar - Gapare W, Hathorn A, Kain D, Matheson C, Wu H:
**Inheritance of spiral grain in the juvenile core of**Pinus radiata**.***Canadian Journal of Forest Research*2007,**37**(1):116–127. 10.1139/x06-202View ArticleGoogle Scholar - Harris JM, Meylan BA:
**The influence of microfibril angle on longitudinal shrinkage and tangential shrinkage in**Pinus radiata**.***Holzforschung*1965,**19:**144–153. 10.1515/hfsg.1965.19.5.144View ArticleGoogle Scholar - Hein PRG, Brancheriau L:
**Radial variation of microfibril angle and wood density and their relationships in 14-year-old**Eucalyptus urophylla**S.T. Blake wood., 6(3), 3352–3362.***BioResources*2011,**6**(3):3352–3362.Google Scholar - Herman M, Dutilleul P, Avella-Shaw T:
**Growth rate effects on intra-ring and inter-ring trajectories of microfibril angle in Norway spruce (**Picea abies**).***IAWA Journal*1999,**20**(1):3–21. 10.1163/22941932-90001542View ArticleGoogle Scholar - Houllier F, Leban J-M, Colin F:
**Linking growth modelling to timber quality assessment for Norway spruce.***Forest Ecology and Management*1995,**74:**91–102. 10.1016/0378-1127(94)03510-4View ArticleGoogle Scholar - Jayawickrama KJS:
**Breeding radiata pine for wood stiffness: review and analysis.***Australian Forestry*2001,**64**(1):51–56. 10.1080/00049158.2001.10676161View ArticleGoogle Scholar - Jordan L, Daniels RF, Clark A, He R:
**Multilevel nonlinear mixed-effects models for the modeling of earlywood and latewood microfibril angle.***Forest Science*2005,**51**(4):357–371.Google Scholar - Jordan L, Re L, Hall DB, Clark AI, Daniels RF:
**Variation in loblolly pine cross-sectional microfibril angle with tree height and physiographic region.***Wood and Fiber Science*2006,**38**(3):390–398.Google Scholar - Jordan L, Re RC, Hall DB, Clark A, Daniels RF:
**Variation in loblolly pine ring microfibril angle in the Southeastern United States.***Wood and Fiber Science*2007,**39**(2):352–363.Google Scholar - Kellomaki S, Peltola H, Ikonen VP:
*Modelling the Structural Growth and Timber Quality of Scots Pine Related to Silvicultural Management*. 1999.Google Scholar - Lasserre JP, Mason EG, Watt MS, Moore JR:
**Influence of initial planting spacing and genotype on microfibril angle, wood density, fibre properties and modulus of elasticity in**Pinus radiata**D. Don corewood.***Forest Ecology and Management*2009,**258**(9):1924–1931. 10.1016/j.foreco.2009.07.028View ArticleGoogle Scholar - Leban JM, Daquitaine R, Houllier F, Saint-Andre L:
**Linking Models for Tree Growth and Wood Quality in Norway Spruce. Part 1: Validations of Predictions for Sawn Properties, Ring Width, Wod Density and Knottiness.***IUFRO Working Party S5.01–04 Workshop Berg-en-Dal, South Africa*1996, 220–228.Google Scholar - Lichtenegger H, Reiterer A, Stanzl-Tschegg SE, Fratzl P:
**Variation of cellulose microfibril angles in softwoods and hardwoods - a possible strategy of mechanical optimization.***Journal of Structural Biology*1999,**128**(3):257–269. 10.1006/jsbi.1999.4194View ArticlePubMedGoogle Scholar - Lindström H, Evans JW, Verrill SP:
**Influence of cambial age and growth conditions on microfibril angle in young Norway spruce (**Picea abies**[L.] Karst.).***Holzforschung*1998,**52**(6):573–581. 10.1515/hfsg.1998.52.6.573View ArticleGoogle Scholar - Lundgren C:
**Microfibril angle and density patterns of fertilized and irrigated Norway spruce.***Silva Fennica*2004,**38**(1):107–117.Google Scholar - Mansfield SD, Parish R, Di Lucca CM, Goudie J, Kang KY, Ott P:
**Revisiting the transition between juvenile and mature wood: a comparison of fibre length, microfibril angle and relative wood density in lodgepole pine.***Holzforschung*2009,**63**(4):449–456. 10.1515/HF.2009.069View ArticleGoogle Scholar - McLean JP, Evans R, Moore JR:
**Predicting the longitudinal modulus of elasticity of Sitka spruce from cellulose orientation and abundance.***Holzforschung*2010,**64:**495–500. 10.1515/hf.2010.084View ArticleGoogle Scholar - Megraw B:
*Longitudinal Shrinkage and Microfibril Angle in Loblolly Pine*. 1998.Google Scholar - Megraw RA, Bremer D, Leaf G, Roers J:
*Stiffness in Loblolly Pine as a Function of Ring Position and Height, and its Relationship to Microfibril Angle and Specific Gravity*. 1999.Google Scholar - Palmer DJ, Cown DJ, Kimberley MO, McKinley RB:
**Assessing prediction accuracy in a regression kriging surface of**Pinus radiata outerwood density across New Zealand**.***Forest Ecology and Management*2013,**308:**9–16. 10.1016/j.foreco.2013.07.024View ArticleGoogle Scholar - Parresol BR:
**Assessing tree and stand biomass: a review with examples and critical comparisons.***Forest Science*1999,**45:**573–593.Google Scholar - Pinheiro J, Bates D, DebRoy S, Sarkar D:
*nlme: Linear and Nonlinear Mixed Effects Models. R Package v.3.1–105*. 2012.Google Scholar - Pinheiro JC, Bates DM:
*Mixed-Effects Models in S and S-PLUS*. Springer, New York; 2000.View ArticleGoogle Scholar - R: a Language and Environment for Statistical Computing. In R Foundation for Statistical Computing (Ed), Vienna; 2013.Google Scholar
- Sarén M-P, Serimaa R, Andersson S, Saranpӓӓ P, Keckes J, Fratzl P:
**Effect of growth rate on mean microfibril angle and cross-sectional shape of tracheids of Norway spruce.***Trees - Structure and Function*2004,**18**(3):354–362. doi:10.1007/s00468–003–0313–8 10.1007/s00468-003-0313-8View ArticleGoogle Scholar - Schimleck LR, Evans R:
**Estimation of microfibril angle of increment cores by near infrared spectroscopy.***IAWA Journal*2002,**23:**225–234. 10.1163/22941932-90000300View ArticleGoogle Scholar - Seifert T:
**Modeling Wood Quality of Norway Spruce (**Picea abies**) Depending on Silvicultural Treatment.***Third IUFRO Workshop "Connection between Silviculture and Wood Quality through Modelling Approaches and Simulation Software", La Londe-Les-Maures, France Sept. 5–12,*1999, 534–540.Google Scholar - Tabet TA, Aziz FA, Abdullah N:
**Modeling microfibril angle and tree age in**Acacia mangium**wood using x-ray diffraction technique.***International Journal of Applied Physics and Mathematics*2012,**2**(5):338–341. 10.7763/IJAPM.2012.V2.128View ArticleGoogle Scholar - Telewski FW:
**Structure and function of flexure wood in**Abies fraseri**.***Tree Physiology*1989,**5:**113–121. 10.1093/treephys/5.1.113View ArticlePubMedGoogle Scholar - Tian X, Cown DJ:
**Modelling wood properties.***New Zealand Forest Service, Forest Research Institute Bulletin No*1995,**201:**72–81.Google Scholar - Vainio U, Andersson S, Serimaa R, Paakkari T, Saranpӓӓ P, Treacy M, Evertsen J:
**Variation of microfibril angle between four provenances of Sitka spruce (**Picea sitchensis**[Bong.] Carr.).***Plant Biology*2002,**4**(1):27–33. 10.1055/s-2002-20433View ArticleGoogle Scholar - Verbelen JP, Stickens D:
**In vivo determination of fibril orientation in plant cell walls with polarisation.***Journal of Microscopy*1995,**177:**1–6. 10.1111/j.1365-2818.1995.tb03528.xView ArticleGoogle Scholar - Wagner L, Bader TK, Auty D, de Borst K:
**Key parameters controlling stiffness variability within trees: a multiscale experimental-numerical approach.***Trees*2012,**27**(1):321–336. doi:10.1007/s00468–012–0801–9 10.1007/s00468-012-0801-9View ArticleGoogle Scholar - Walker JCF, Butterfield B:
**The importance of microfibril angle for the processing industries.***New Zealand Journal of Forestry*1995,**40**(4):34–40.Google Scholar - Walker JFC:
**The importance of microfibril angle for the processing industries.***New Zealand Journal of Forestry*1996,**40**(4):34–40.Google Scholar - Wang M, Stewart JD:
**Determining the transition from juvenile to mature wood microfibril angle in lodgepole pine: a comparison of six different two-segment models.***Annals of Forest Science*2012,**69**(8):927–937. doi:10.1007/s13595–012–0226-z 10.1007/s13595-012-0226-zView ArticleGoogle Scholar - Wardrop AB, Preston RD:
**Organisation of the cell walls of tracheids and wood fibres.***Nature*1947,**160:**911–913. 10.1038/160911a0View ArticlePubMedGoogle Scholar - Watt MS, Zoric B:
**Development of a model describing modulus of elasticity across environmental and stand density gradients in plantation-grown Pinus radiata within New Zealand.***Canadian Journal of Forest Research*2010,**40**(8):1558–1566. 10.1139/X10-103View ArticleGoogle Scholar - Watt MS, Zoric B, Kimberley MO, Harrington J:
**Influence of stocking on radial and longitudinal variation in modulus of elasticity, microfibril angle, and density in a 24-year-old**Pinus radiata**thinning trial.***Canadian Journal of Forest Research*2011,**41**(7):1422–1431. doi:10.1139/x11–070 10.1139/x11-070View ArticleGoogle Scholar - West GG:
**Standpak evaluation of the effects of site, silviculture, and genetics on mean log age and the proportion of juvenile wood.***New Zealand Journal of Forestry Science*1997,**27:**324–342.Google Scholar - West GG, Moore JR, Shula RG, Harrington JJ, Snook J, Gordon JA, Riordan MP:
**Forest Management DSS Development in New Zealand.**In*Implementation of DSS Tools into the Forestry Practice*. Edited by: Tucek J, Smrecek R, Majlingova A, Garcia-Gonzalo J. Technical University of Zvolen, Slovakia; 2013:153–163.Google Scholar - Wimmer R, Downes GM, Evans R:
**Temporal variation of microfibril angle in**Eucalyptus nitens**grown in different irrigation regimes.***Tree Physiology*2002,**22**(7):449–457. 10.1093/treephys/22.7.449View ArticlePubMedGoogle Scholar - Wu HX, Ivković M, Gapare WJ, Matheson AC, Baltunis BS, Powell MB, McRae TA:
**Breeding for wood quality and profit in**Pinus radiata**: a review of genetic parameter estimates and implications for breeding and deployment.***New Zealand Journal of Forestry Science*2008,**38**(1):56–87.Google Scholar - Xu P, Walker JCF:
**Stiffness gradients in radiata pine trees.***Wood Science and Technology*2004,**38**(1):1–9. 10.1007/s00226-003-0188-2View ArticleGoogle Scholar - Zobel BJ, Sprague JR:
*Juvenile Wood in Forest Trees*. Springer, Berlin; 1998.View ArticleGoogle Scholar - Katz A, Dunningham A, Gordon A:
*A Compatible Volume and Taper Equation for New Zealand Pinus Radiata D. Don Grown Under the Direct Sawlog Regime. (FRI Bulletin No. 67)*. Forest Research Institute, New Zealand Forest Service, Rotorua, New Zealand; 1984.Google Scholar

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.